Gold nanoarray deposited using alternating current for emission rate-manipulating nanoantenna
© Xue et al.; licensee Springer. 2013
Received: 30 April 2013
Accepted: 18 June 2013
Published: 24 June 2013
We have proposed an easy and controllable method to prepare highly ordered Au nanoarray by pulse alternating current deposition in anodic aluminum oxide template. Using the ultraviolet–visible-near-infrared region spectrophotometer, finite difference time domain, and Green function method, we experimentally and theoretically investigated the surface plasmon resonance, electric field distribution, and local density of states enhancement of the uniform Au nanoarray system. The time-resolved photoluminescence spectra of quantum dots show that the emission rate increased from 0.0429 to 0.5 ns−1 (10.7 times larger) by the existence of the Au nanoarray. Our findings not only suggest a convenient method for ordered nanoarray growth but also prove the utilization of the Au nanoarray for light emission-manipulating antennas, which can help build various functional plasmonic nanodevices.
82.45.Yz, 78.47.jd, 62.23.Pq
Excited by an incident photon beam and provoking a collective oscillation of free electron gas, plasmonic materials gain the ability to manipulate electromagnetic field at a deep-subwavelength scale, making them play a major role in current nanoscience [1–5]. The plasmonic metallic nanostructures have presented a vast number of potential applications in various prospective regions such as plasmon lasers [6–8], optical tweezers [9, 10], and biochemical sensing platforms [11–13]. In particular, the nanoarray structure attracts extensive research efforts for its strong coupling between adjacent nanorods, which leads to dramatic field enhancement and high energy transfer efficiency [14, 15], resulting in a diverse range of plasmonic devices such as subwavelength color imaging, plasmonic waveguide, functional metamaterials [15–19], as well as nanoantennas for manipulating the light emission of various nanoemitters, which is of great importance for quantum science, nano-optical communication, and light-harvesting devices [20–25].
Owing to the self-organized hexagonal arrays of uniform parallel nanochannels, anodic aluminum oxide (AAO) film has been widely used as the template for nanoarray growth [26–29]. Many distinctive discoveries have been made in the nanosystems fabricated in AAO films [30–34]. As increasing emphasis is placed on low cost, high throughput, and ease of production, AAO template-assisted nanoarray synthesis is becoming the method of choice for the fabrication of nanoarrays .
However, due to the existence of a barrier layer, it is impossible to grow nanoarrays instantly after the AAO template has been prepared via a two-step anodization process using direct current (DC). Some complicated processes must be included, such as the Al foil removing, the barrier layer etching, and the conducting layer making. The pregrowth processes dramatically increase the difficulty of AAO template-assisted nanoarray synthesis especially in the case that a thin AAO film with a few micrometer is required . On the other hand, it is reported that alternating current (AC) can get across the barrier layer and implement direct metal array deposition [36–38]. However, using the AC method, it is difficult to grow the nanoarray as ordered as that using DC, which leads to poor field enhancement and broad surface plasmon resonance (SPR) peaks [18, 36–38]. This flaw prevents the AC growth method from being widely used.
In this paper, we propose a pulse AC metal nanoarray growth method, which can cut off some inevitable complicated processes in AAO DC deposition and easily fabricate metallic nanoarrays as uniform as those by DC deposition. The extinction spectra, the quantum dot (QD) emission rate manipulation measurement, as well as the theoretical analysis of electric field distribution and local density of states (LDOS) confirm that the pulse AC-grown Au nanoarrays can be a good candidate for nanoantennas.
Preparation of samples
The AAO templates were prepared by a two-step anodization process [18, 33]. First, the aluminum sheets (purity 99.999%) were degreased in acetone and electropolished under a constant current condition of 1.2 A for 3 min in a mixture of HClO4 and C2H5OH at 0°C to smooth the surface morphology. In the first and second anodization processes, treated aluminum sheets were exposed to 0.3 M H2SO4 or H2C2O4 solution under a constant voltage of 19 or 45 V in an electrochemical cell at a temperature of about 4°C. The alumina layer produced by the first anodization process was removed by wet chemical etching in a mixture of phosphoric acid (0.15 M) and chromic acid (0.60 M) at 60°C for 1 h. The barrier layer of AAO templates was thinned stepwise with reducing potential down to 6 V.
The ordered Au nanoarrays were deposited in the nanopores of the AAO template by pulse AC (50 Hz) electrodeposition in an electrolyte containing HAuCl4 (10 mM) and H2SO4 acid (0.03 M) with a Pt counter electrode. The deposition was carried on instantly after the completion of the AAO template using a common AC power source (GW APS-9301, GW Instek, New Taipei City, Taiwan) supplying a 4-s pulse of 16 V, followed by a growth potential of 9 V. There is no need to remove the Al foil, etch the barrier layer, and make a conducting layer before Au nanoarray growth, which makes the electrodeposition very convenient. The normal AC deposition method was carried on in the same condition as the pulse AC, except for the 4-s pulse of 16 V.
The quantum dots were commercial carboxyl CdSe/ZnS quantum dots, which were purchased from Invitrogen Corporation (Carlsbad, CA, USA). In the time-resolved photoluminescence (PL) measurement of the QDs, the Al foil was taken using CuCl2 solution, and QDs were dropped on the barrier side of the AAO template.
Characterization of samples
Scanning electron microscopy (SEM) was performed using a Zeiss Auriga-39-34 (Oberkochen, Germany) operated at an accelerating voltage of 5.0 kV. Transmission electron microscopy (TEM) was performed using a JEOL 2010HT (Akishima-shi, Japan) operated at 100 kV. The TEM samples were prepared by dissolving the AAO template containing Au nanoarrays in NaOH solution. The extinction spectra were recorded using an ultraviolet–visible-near-infrared region (UV–vis-NIR) spectrophotometer (PerkinElmer Lambda950, Waltham, MA, USA) using a p-polarized source with an incident angle of 70°.
The PL from the samples was collected by the reflection measurement. An s-polarized laser for the measurements of PL was generated using a mode-locked Ti:sapphire laser (MaiTai, Spectra Physics, Newport Corporation, Irvine, CA, USA) with a pulse width of approximately 150 fs and a repetition rate of 79 MHz. The wavelength of the laser beam was tuned to 400 nm. The scattering noise was filtered using a band-pass filter, followed by a 100-mm-focal-length lens which was used to excite the sample at a Brewster angle θb ≈ 50°. The luminescence from the sample was collected using the focusing lens and a long-wave pass filter before entering the liquid-nitrogen-cooled CCD (SPEC-10, Princeton Instruments, Trenton, NJ, USA). The time-resolved PL decay traces were recorded using a time-correlated single-photon counting system (PicoQuant GmbH, Berlin, Germany).
The computational simulations were performed using the finite difference time domain (FDTD) method with Bloch and perfectly matched layer (PML) boundary conditions for the x- and y- axes and z-axis, respectively. The cell size was 2 × 2 × 5 nm3. The nanowires were hexagonally arrayed with a rod diameter of 34 nm, length of 150 nm, and spacing of 110 nm. The refractive index of Al2O3 was set to be 1.76, and the complex dielectric constants of the gold were taken from the literature of Johnson and Christy .
The photonic LDOS was obtained by calculating the Green function with the help of the COMSOL software (version 4.2a). The hexagonal lattice of Au nanowires was simulated with the scale of 7 × 7 arrays. The lattice constant was set to be 110 nm. The length and the diameter of each Au nanowire were set to be 150 and 34 nm, respectively. The refractive index of the background was 1.76. The dielectric constant of gold was taken from the literature of Johnson and Christy . An electric point dipole is set 10 nm above the center of the arrays. A block with the size of 0.99 × 0.887 × 0.31 μm3 is set to separate the array and the PML. The PML is set to a size of 1.65 × 1.547 × 1.15 μm3 with general type. To get a good mesh, a sphere with the radius of 4 nm is set to surround the dipole. The mesh inside the block is predefined as fine. The mesh of the PML is predefined as extra fine to get good absorption. The scattering boundary is set to the outside of the PML.
Results and discussion
The inset of Figure 1a is the cross-sectional SEM view of the AAO template made in H2C2O4. It can be seen that the nanochannels are very vertical, which makes it possible to grow highly ordered nanoarrays. The TEM image of Au nanowires is presented in the inset of Figure 1b. These Au nanowires were grown in the AAO template manufactured by H2C2O4 anodization, with the average diameter and length being 34 and 150 nm, respectively. It should be noted that the Au nanowires in the inset TEM image were deposited by the pulse AC method, which made the highly ordered growth possible. On the other hand, the good length uniformity as well as high occupied rate can hardly be achieved using the normal AC method (see Additional file 1: Figures S1 and S2).
To further discuss the extinction spectra results, we used the FDTD method to calculate the extinction spectra of uniform and nonuniform nanoarrays (Figure 2c). The length of a single nanowire in the uniform Au nanoarray is set to be 150 nm according to TEM images, and the basic simulation unit cell of the nonuniform Au array contains six nanowires with the length L = 50, 75, 100, 125, 150, and 200 nm (simulation model, see Additional file 1: Figure S3). From Figure 2c, it is obviously seen that the extinction intensity ratio of LSPRs to TSPRs decreases dramatically in the nonuniform nanoarray structure (blue curve), and this phenomenon fits quite well with the experimental result. There are several LSPR peaks appearing at the nonuniform nanoarray extinction spectra, which are caused by the LSPRs of Au nanowires with different length. For the normal AC-grown nanoarrays, the length of a single Au nanowire varies continuatively, so numerous LSPR peaks can finally broaden the FWHM of the Au nanoarray extinction spectra. Furthermore, it is interesting to note that the LSPR location of simulation data fits quite well with the experimental results (788 nm in experiment, 792 nm in simulation). Due to the strong SPRs in the pulse AC-grown Au nanoarray, it is believed that the uniform Au nanoarray can generate large enhancement of electric field and local density of states, which makes the Au nanoarray a good candidate for nanoantennas. Thus, we use the FDTD and Green function methods to do our further theoretical investigation.
From the Maxwell equations, one can get By setting a dipole source the Green function can be calculated by the electric field at the position of the dipole as .
After choosing three of different directions, all the elements of the Green matrix can be obtained so as to get the LDOS.
The LDOS is calculated by the finite element method with the help of the COMSOL software (version 4.2a). As shown in Figure 3b, one can see that the LDOS enhancement at 792 nm is much larger at the edge which is in accord with the field distribution in Figure 3a, and the maximum enhancement is 81.2 times (define the LDOS enhancement as the ratio of LDOS around the nanoarray to LDOS in vacuum). The z-position dependence of LDOS enhancement shows that the LDOS enhancement decreases dramatically with the increase of distance at the z-axis, and the LDOS enhancement phenomenon nearly disappears at the point of 50 nm above (see Figure 3c). If we can control the z-distance between the nanoemitter and the Au nanoarray, it is possible to manipulate the LDOS enhancement as well as the light emission rate. Moreover, the large field and LDOS enhancement can also be demonstrated by the PL measurement [33, 45], and these detailed experimental results can be found in Additional file 1: Figure S4.
From the data in Figure 4, ts is 23.3 ns, while tf is 2.0 and 3.4 ns for QDs on uniform and nonuniform Au nanoarrays, respectively. As the enhancement of LDOS decreases dramatically with the increase of distance (see Figure 3c), the slow decay process may indicate a part of the QDs which are quite far from the Au nanoarray, and the fast decay process can be attributed to the QDs that are located at the LDOS-enhancing region. From the fitting data, the emission rate of the QDs on the uniform Au nanoarray increased from 0.0429 to 0.50 ns−1, showing an enhancement of 10.7 times. As the distance between QDs and Au nanoarray is variable (QDs cannot assemble at the top side of the Au nanoarray) and the LDOS enhancement is sensitive to the increase of the z distance, it is reasonable that the light emission rate enhancement is smaller than the average theoretical LDOS enhancement. Also, it should be noted that the normalized Af rate (Af / (Af + As)) for QDs on uniform and nonuniform Au nanoarrays is 87.4% and 76.1%, which means that the fast decay process is dominant and the uniform Au nanoarray is a better choice for emission-manipulating nanoantennas. This Au nanoarray is the sample in Figure 2b, which is similar to the uniform simulation model of Figure 3, and the time-resolved PL spectra of QDs with emission peak located at 790 nm on the Au nanoarray can be found in Additional file 1: Figure S5.
In this letter, we have proposed an easy and controllable method to prepare highly ordered Au nanoarrays by pulse alternating current deposition in anodic aluminum oxide template. This method not only averts some complicated inevitable processes in AAO DC deposition but also can easily fabricate Au nanoarrays as uniform as those by the DC deposition, which can be demonstrated using SEM image, TEM image, and UV–vis-NIR spectrophotometer. Using the FDTD and Green function methods, we further theoretically investigated the surface plasmon resonance, electric field distribution, and LDOS enhancement in the uniform Au nanoarray system and found that the maximum LDOS enhancement can be 81.2 times at the tip of the Au nanoarray. The time-resolved PL spectra of quantum dots show that the Au nanoarray can increase the emission rate of QDs from 0.0429 to 0.5 ns−1 (10.7 times larger). Our findings reveal that the conveniently AC-grown Au nanoarray can serve as light emission-manipulating antennas and could help build various functional plasmonic nanodevices.
Anodic aluminum oxide
Finite difference time domain
Full width at half maximum
Local density of states
Perfectly matched layers
Scanning electron microscopy
Surface plasmon resonance.
This work was supported in part by NSFC (11204385), the National Basic Research Program of China (2010CB923200), the Fundamental Research Funds for the Central Universities (grant 12lgpy45), and a fund from the Education Department of Guangdong Province (2012LYM_0011).
- Liu N, Hentshel M, Weiss T, Alivisatos A, Giessen H: Three-dimensional plasmon rulers. Science 2011, 322: 1407–1410.View ArticleGoogle Scholar
- Chen HJ, Shao L, Li Q, Wang JF: Gold nanorods and their plasmonic properties. Chem Soc Rev 2013, 42: 2679–2724. 10.1039/c2cs35367aView ArticleGoogle Scholar
- Schmidt M, Lei DY, Wondraczek L, Nazabal V, Maier S: Hybrid nanoparticle–microcavity-based plasmonic nanosensors with improved detection resolution and extended remote-sensing ability. Nat Comm 2012, 3: 1108.View ArticleGoogle Scholar
- Lal S, Link S, Halas N: Nano-optics from sensing to waveguiding. Nat Photonics 2007, 1: 641–648. 10.1038/nphoton.2007.223View ArticleGoogle Scholar
- Martin-Cano D, Martin-Moreno L, García-Vidal F, Moreno E: Resonance energy transfer and superradiance mediated by plasmonic nanowaveguides. Nano Lett 2010, 10: 3129–3134. 10.1021/nl101876fView ArticleGoogle Scholar
- Sorger V, Zhang X: Spotlight on plasmon lasers. Science 2011, 333: 709–710. 10.1126/science.1204862View ArticleGoogle Scholar
- Russell K, Liu TL, Cui S, Hu EL: Large spontaneous emission enhancement in plasmonic nanocavities. Nat Photonics 2012, 6: 459–462. 10.1038/nphoton.2012.112View ArticleGoogle Scholar
- Noginov M, Zhu G, Belgrave A, Bakker R, Shalaev V, Narimanov E, Stout S, Herz E, Suteewong T, Wiesner U: Demonstration of a spaser-based nanolaser. Nature 2009, 460: 1110–1113. 10.1038/nature08318View ArticleGoogle Scholar
- Juan ML, Righini M, Quidant R: Plasmon nano-optical tweezers. Nat Photonics 2011, 5: 349–356. 10.1038/nphoton.2011.56View ArticleGoogle Scholar
- Schuller J, Barnard E, Cai W, Jun YC, White J, Brongersma M: Plasmonics for extreme light concentration and manipulation. Nat Mater 2010, 9: 193–204. 10.1038/nmat2630View ArticleGoogle Scholar
- Fan J, Wu C, Bao K, Bao J, Bardhan R, Halas N, Manoharan V, Nordlander P, Shvets G, Capasso F: Self-assembled plasmonic nanoparticle clusters. Science 2010, 328: 1135–1138. 10.1126/science.1187949View ArticleGoogle Scholar
- Reed J, Zhu H, Zhu AY, Li C, Cubukcu E: Graphene-enabled silver nanoantenna sensors. Nano Lett 2012, 12: 4090–4094. 10.1021/nl301555tView ArticleGoogle Scholar
- Li JF, Huang YF, Ding Y, Yang ZL, Li SB, Zhou XS, Fan FR, Zhang W, Zhou ZY, Wu DY, Ren B, Wang ZL, Tian ZQ: Shell-isolated nanoparticle-enhanced Raman spectroscopy. Nature 2010, 464: 392–395. 10.1038/nature08907View ArticleGoogle Scholar
- Evans P, Kullock R, Hendren W, Atkinson R, Pollard R, Eng L: Optical transmission properties and electric field distribution of interacting 2D silver nanorod arrays. Adv Funct Mater 2008, 18: 1075–1079. 10.1002/adfm.200701289View ArticleGoogle Scholar
- Liu SD, Cheng MT, Yang ZJ, Wang QQ: Surface plasmon propagation in a pair of metal nanowires coupled to a nanosized optical emitter. Opt Lett 2008, 33: 851–853. 10.1364/OL.33.000851View ArticleGoogle Scholar
- Kawata S, Ono A, Verma P: Subwavelength colour imaging with a metallic nanolens. Nat Photonics 2008, 2: 438–442. 10.1038/nphoton.2008.103View ArticleGoogle Scholar
- Lyvers D, Moon J, Kildishev A, Shalaev V, Wei A: Gold nanorod arrays as plasmonic cavity resonators. ACS Nano 2008, 2: 2569–2576. 10.1021/nn8006477View ArticleGoogle Scholar
- Zhou ZK, Li M, Yang ZJ, Peng XN, Su XR, Zhang ZS, Li JB, Kim N, Yu XF, Zhou L, Hao ZH, Wang QQ: Plasmon-mediated radiative energy transfer across a silver nanowire array via resonant transmission and subwavelength imaging. ACS Nano 2010, 4: 5003–5010. 10.1021/nn100578bView ArticleGoogle Scholar
- Yao J, Liu Z, Liu Y, Wang Y, Sun C, Bartal G, Stacy A, Zhang X: Optical negative refraction in bulk metamaterials of nanowires. Science 2008, 321: 930–930. 10.1126/science.1157566View ArticleGoogle Scholar
- Mühlschlegel P, Eisler J, Martin O, Hecht B, Pohl D: Resonant optical antennas. Science 2005, 308: 1607–1609. 10.1126/science.1111886View ArticleGoogle Scholar
- Knight M, Sobhani H, Nordlander P, Halas N: Photodetection with active optical antennas. Science 2011, 332: 702–704. 10.1126/science.1203056View ArticleGoogle Scholar
- Novotny L, van Hulst N: Antennas for light. Nat Photonics 2011, 5(2):83–90. 10.1038/nphoton.2010.237View ArticleGoogle Scholar
- Novotny L: Effective wavelength scaling for optical antennas. Phys Rev Lett 2007, 98: 266802.View ArticleGoogle Scholar
- Righini M, Ghenuche P, Cherukulappurath S, Myroshnychenko V, García de Abajo F, Quidant R: Nano-optical trapping of Rayleigh particles and Escherichia coli bacteria with resonant optical antennas. Nano Lett 2009, 9: 3387–3391. 10.1021/nl803677xView ArticleGoogle Scholar
- Acar H, Coenen T, Polman A, Kuipers L: Dispersive ground plane core-shell type optical monopole antennas fabricated with electron beam induced deposition. ACS Nano 2012, 6: 8226–8232. 10.1021/nn302907jView ArticleGoogle Scholar
- Masuda H, Fukuda K: Ordered metal nanohole arrays made by a two-step replication of honeycomb structures of anodic alumina. Science 1995, 268: 1466–1468. 10.1126/science.268.5216.1466View ArticleGoogle Scholar
- Lee W, Ji R, Gösele U, Nielsch K: Fast fabrication of long-range ordered porous alumina membranes by hard anodization. Nat Mater 2006, 5: 741–747. 10.1038/nmat1717View ArticleGoogle Scholar
- Lee W, Schwirn K, Steinhart M, Pippel E, Scholz R, Gösele U: Structural engineering of nanoporous anodic aluminium oxide by pulse anodization of aluminium. Nat Nanotechnol 2008, 3: 234–239. 10.1038/nnano.2008.54View ArticleGoogle Scholar
- Rycenga M, Cobley C, Zeng J, Li W, Moran C, Zhang Q, Qin D, Xia Y: Controlling the synthesis and assembly of silver nanostructures for plasmonic applications. Chem Rev 2011, 111: 3669–3712. 10.1021/cr100275dView ArticleGoogle Scholar
- Ji N, Ruan WD, Wang CX, Lu ZC, Zhao B: Fabrication of silver decorated anodic aluminum oxide substrate and its optical properties on surface-enhanced Raman scattering and thin film interference. Langmuir 2009, 25: 11869–11873. 10.1021/la901521jView ArticleGoogle Scholar
- Banerjee P, Perez I, Henn-Lecordier L, Lee B, Rubloff G: Nanotubular metal–insulator–metal capacitor arrays for energy storage. Nat Nanotechnol 2009, 4: 292–296. 10.1038/nnano.2009.37View ArticleGoogle Scholar
- Park S, Taton T, Mirkin C: Array-based electrical detection of DNA with nanoparticle probes. Science 2002, 295: 1503–1506.View ArticleGoogle Scholar
- Zhou ZK, Peng XN, Yang ZJ, Zhang ZS, Li M, Su XR, Zhang Q, Shan X, Wang QQ, Zhang Z: Tuning gold nanorod-nanoparticle hybrids into plasmonic Fano resonance for dramatically enhanced light emission and transmission. Nano Lett 2011, 11: 49–55. 10.1021/nl1026869View ArticleGoogle Scholar
- Zhao SY, Roberge H, Yelon A, Veres T: New application of AAO template: a mold for nanoring and nanocone arrays. J Am Chem Soc 2006, 128: 12352–12353. 10.1021/ja062148+View ArticleGoogle Scholar
- Hurst S, Payne E, Qin LD, Mirkin C: Multisegmented one-dimensional nanorods prepared by hard-template synthetic methods. Angew Chem Int Ed 2006, 45: 2672–2692. 10.1002/anie.200504025View ArticleGoogle Scholar
- Giallongo G, Durante C, Pilot R, Garoli D, Bozio R, Romanato F, Gennaro A, Rizzi G, Granozzi G: Growth and optical properties of silver nanostructures obtained on connected anodic aluminum oxide templates. Nanotechnology 2012, 23: 325604. 10.1088/0957-4484/23/32/325604View ArticleGoogle Scholar
- Peng XN, Zhou ZK, Zhang W, Hao ZH: Dynamically tuning emission band of CdSe/ZnS quantum dots assembled on Ag nanorod array: plasmon-enhanced Stark shift. Opt Express 2011, 19: 24804–24809. 10.1364/OE.19.024804View ArticleGoogle Scholar
- Zhou ZK, Su XR, Peng XN, Zhou L: Sublinear and superlinear photoluminescence from Nd doped anodic aluminum oxide templates loaded with Ag nanowires. Opt Express 2008, 16: 18028–18033. 10.1364/OE.16.018028View ArticleGoogle Scholar
- Johnson P, Christy R: Optical constants of the noble metals. Phys Rev B 1972, 6: 4370–4379. 10.1103/PhysRevB.6.4370View ArticleGoogle Scholar
- Kabashin AV, Evans P, Pastkovsky S, Hendren W, Wurtz GA, Atkinson R, Pollard R, Podolshiy VA, Zayats AV: Plasmonc nanorod metamaterials for biosensing. Nat. Mater. 2009, 8: 867–871. 10.1038/nmat2546View ArticleGoogle Scholar
- Wurtz G, Pollard R, Hendren W, Wiederrecht G, Gosztola D, Podolskiy V, Zayats A: Designed ultrafast optical nonlinearity in a plasmonic nanorod metamaterial enhanced by nonlocality. Nat Nanotechnol 2011, 6: 106–110.View ArticleGoogle Scholar
- Pollard R, Murphy A, Hendren W, Evans P, Atkinson R, Wurtz G, Zayats A: Optical nonlocalities and additional waves in epsilon-near-zero metamaterials. Phys Rev Lett 2009, 102: 127405.View ArticleGoogle Scholar
- Nielsch K, Müller F, Li AP, Gösele U: Uniform nickel deposition into ordered alumina pores by pulsed electrodeposition. Adv Mater 2000, 12: 582–586. 10.1002/(SICI)1521-4095(200004)12:8<582::AID-ADMA582>3.0.CO;2-3View ArticleGoogle Scholar
- Novotny L, Hecht B: Principles of Nano-optics. Cambridge: Cambridge University Press; 2006.View ArticleGoogle Scholar
- Wang QQ, Han JB, Guo DL, Xiao S, Han YB, Gong HM, Zou XW: Highly efficient avalanche multiphoton luminescence from coupled Au nanowires in the visible region. Nano Lett 2007, 7: 723–728. 10.1021/nl062964fView ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.